Download Chapter 17old...
17 Soft Magnetic Materials Soft magnetic materials are used extensively in power electronic circuits, as voltage and current transformers, saturable reactors, magnetic amplifiers, inductors, and chokes. These magnetic devices may be required to operate at only 50/60 Hz, or at frequencies down to dc or over 1 MHz. For example, a steel lamination ac mains voltage transformer operates at 50/60 Hz, while its ferrite switch-mode power supply equivalent may operate at 500 kHz. Soft magnetic materials have been utilised in other chapters for the following applications: switching aid circuits - linear inductor (8.3.3) - saturable inductor (8.3.4) - snubber discharge (figure 8.5) - unified energy recovery (9.2.1) - thyristor di/dt control (figure 8.5) pulse transformers (figures 7.7f) current transformer turn-on snubber energy recovery (figures 9.2a) L-C resonator circuits (figure 9.5c) transient current sharing (figure 10.8) rfi filtering (10.4.2) single and three phase transformers (11, 12) cycloconverter intergroup reactors (12.5) phase shifting transformers (14.1.3ii) current source inductance (14.2) smps inductance and transformers (15) Hard magnetic materials, which are used for permanent magnets and ferrite beads for rfi suppression, are not specifically considered. 17.1
Two basic types of soft magnetic materials are extensively used, depending on the application and its requirements. These materials are:
Ferromagnetic materials based on iron and nickel, which are for lower frequencies, < 2kHz, while Ferrimagnetic materials, which are based on ceramic oxides of metals, are applicable to frequencies from a few kilohertz to well over 80 MHz. Ferromagnetic materials
17.1.1i - Steel Cold-rolled grain-oriented steel is a 3-4 per cent silicon iron, cold reduced to develop a high degree of grain orientation, which gives • increased flux for a given magnetising force and • decreased size for a given rating, hence reduced weight. Normally cores are produced in a number of material lamination thicknesses • 0.3 mm for frequencies up to 200 Hz • 0.1 mm for frequencies between 200 Hz to 2 kHz and • 0.05 mm for higher frequencies and pulse applications. Steel laminations for low frequency applications are available in different shapes. E and I laminations or strip C cores or toroids are extensively used for mains transformers and ac line inductors. Non-orientated silicon steels are extensively used for machine laminations. 17.1.1ii - Iron powders Two general forms of iron powder cores are employed • •
Cores are made by highly compacting insulated high quality spongy iron powder. High resistivity is required to reduce eddy current losses and so the iron powder is subjected to an acid treatment to produce an insulating oxide layer on the surface of each individual particle. This fine carbonyl iron is mixed with a bonding material and highly compressed. The bonding material used limits the maximum core temperature. Minute gaps appear between the particles, severely reducing the permeability. It is difficult to saturate such materials.
17.1.1iii - Alloy powders These cores are made by highly compacting insulated alloy powder. The alloy is usually 50-75 per cent nickel, the remainder being iron with a small percentage of copper and molybdenum. The higher the iron percentage, the higher the saturation flux density and the higher the losses.
Soft Magnetic materials
Powder iron and alloy cores are available in toroidal or ring shapes, cylindrical and hollow cylindrical cores, as well as cup cores, bobbins, pot cores, and beads. 17.1.2
Power Electronics Table 17.1. Typical comparative data of soft magnetic materials
Frequency range, ∆f
Temperature range, ∆T
Initial permeability, µi flux density, Bs @ 25°C
Table 17.1 shows typical comparative data for the main classes of soft ferro and ferri magnetic materials. Generally, those materials with higher saturating flux densities, Bs, have higher initial permeability µi, and hence offer higher inductance but at the expense of higher core eddy current and hysteresis losses. Typical B-H curve characteristics are shown in figure 17.1 for the different soft magnetic materials shown in table 17.1. In the case of a transformer, the advantage of a high core flux density is that more volts v, per turn N, for a given frequency f, results. This is seen from Faraday’s Law: dφ dB (17.1) v=N = NA (V) dt dt whence for sinusoidal flux (17.2) v = 4.44 NBs Ae f (V)
Ferrites Mn-Zn Ni-Zn
-55 to 300 -55 to 125 -55 to 105 -55 to 200 -30 to 105
T remanence, Br Intrinsic mmf strength A/m Hi = (Bs - Br)/2µi Ωcm Resistivity, ρ
Curie temperature, Tc
-55 to 250
Inductance is specified from equation (17.1) and from di v=L (V) dt dφ L=N (H) di Using φ = BAe and Hℓe = Ni, equation (17.4) becomes L=
17.2 Comparison of material types
Iron powder carbonyl
Ferrimagnetic materials - soft ferrites
Ferrites are black, hard, brittle, chemically inert ceramic materials, which have a magnetic cubic structure. The most general ferrites are polycrystalline magnetic ceramic oxides, which are compounds of iron oxide, Fe203 mixed with one or more oxides of bivalent transition metals such as Fe0, Ni0, Zn0, Mn0, Cu0, Ba0, Co0, and Mg0. At lower frequencies, below a few MHz, a Mn-Zn combination is added to iron oxide, while for higher frequencies, above a MHz, Ni-Zn is the additive. The raw oxide materials are mixed, pre-sintered at 1000°C if required, and ground. The powder material is shaped by means of pressing and sintering at between 1150°C and 1300°C. The sintering process involves raising the temperature to 1300°C in about 3 h, with 15 per cent oxygen present. The cores are cooled slowly without oxygen present to about 200°C in 20 h after entry. A 15 per cent linear, and 40 per cent by volume shrinkage occurs during sintering. A diverse range of ferrite core shapes is available, which include, E, I, U, toroid, drum, pot, rod, tube, and screw. Where appropriate, diamond-wheel-ground air gaps are available on the centre pole. Manufacturing yields limit the physical component in size. Toroid cores of 152 mm outside diameter are not uncommon, and exotic shapes such as motor stators are made for special applications.
N 2 Ae dB e
105 - 106
where dB/dH is the slope of the B-H curve, according to B = µoµiH. Therefore, before core saturation N 2 Ae (17.6) L= µ o µi (H) e
The subscript e is used to denote the effective core parameter, as shown in table 17.2. In rfi suppression and filtering applications, silicon steel is not effective since the initial permeability, µi, falls rapidly with frequency hence at the high suppression frequency, inductance is small. Thus iron powder or a high iron alloy may be used, which have relatively high flux densities and high losses. For rfi suppression, a high core loss aids suppression. At inaudible frequencies, >20 kHz, for a low core loss, ferrites are extensively used. Although ferrite flux densities are relatively low, typically 0.4 T, eddy current and hysteresis losses are low. The low eddy current loss results from the high core material resistivity. With ferromagnetic materials, the eddy current loss is reduced by using thinner laminations or electrically isolated powder particles. A major disadvantage of a ferrite core is its poor temperature stability and low allowable core temperature. On the other hand, high initial permeabilities, >12,000, are obtainable.
Soft Magnetic materials
Table 17.2. Core effective dimensions and parameters
Ferrite materials, application, and component design are specifically considered, although the concepts developed are generally applicable to ferromagnetic materials.
core factor -1
c1 / Σℓ/A
From the parameters in table 17.2, inductance is calculated from equation (17.6) as L = µi cN 2 (H) (17.7)
Figure 17.1 shows that a non-linear relationship exists between B and H for magnetic materials, and is characterised by the dimensionless parameter µr - the relative permeability - according to B = µo µr H (where µo = 4π×10-7 H/m). Figure 17.2 shows a detailed B-H magnetising curve for a ferrite material along with its hysteresis loop. The case of an air core magnetic circuit, for which µr = 1, is also shown. Figure 17.2 illustrates various definitions for µr based on 1 B (17.8) µr = µo H Figure 17.1. Magnetisation curves for soft magnetic materials.
The definitions and explanations given are applicable to soft magnetic materials in general and are illustrated specifically by reference to ferrite materials. General mechanical and thermal properties of ferrites are given in appendix 17.6.
Dimensions and parameters
The effective magnetic dimensions are constant for a given core and are defined in table 17.2. These effective constants are based on the length ℓ and area A of the individual limbs comprising the complete core. These effective dimensions are used for magnetic component design, such as transformer core loss, which is given per unit effective volume, Ve.
17.3.2i - Initial permeability, µi The initial permeability, which is dependant on temperature and frequency, is the permeability at weak field strengths at H = 0 and ∆H tends to zero, that is 1 ∆B (17.9) µi = µo ∆H H = 0, ∆H → 0 ∧
17.3.2ii - Amplitude permeability, µa and maximum permeability, µ The amplitude permeability applies to large magnitude sinusoids, with no dc field applied, and is the ratio of the sinusoid peak B and H 1 B (17.10) µa = µo H H = 0 ∧ ∧ µ is the maximum µa obtainable for any H, that is, µ = max [µa] for all values of H. The variation of amplitude permeability with magnetising force or flux density is shown in figure 17.3. Because of the non-linear nature of the B-H curve loop, the amplitude permeability is highly dependant of the applied field strength magnitude.
Soft Magnetic materials
This figure 17.3 is representative of a ferrite material suitable for a wide range of power electronic applications. More technical data for this material is presented in Appendix 17.7 and in the figures that follow.
µ∆ µ o
µo ∆H → 0 ∆H
H = constant
The incremental permeability, µ∆ is a function of the dc magnetic bias, as shown in figure 17.4. It is usually a maximum when no dc field is present, while for a toroid it is identical with the initial permeability, µi. With increased current, µ∆, hence inductance, decreases.
µa µ o
Figure 17.2. Hysteresis loop illustrating permeability definitions, remanence Br, and coercive force Hc.
17.3.2iii - Reversible or incremental permeability, µrev, µ∆ When a core is magnetised with a polarising dc offset field upon which a small ac field is superimposed, the ac H field produces a small lancet-shape hysteresis loop which reduces to a straight line as the ac H field is reduced. The slope of this line, shown in figure 17.2, is called the incremental or reversible permeability
Figure 17.3. Temperature dependence of flux density and permeability, µa.
Soft Magnetic materials
17.3.2iv - Effective permeability, µe The inductance of a coil with a gapped core of effective permeability µe is given by µ µ N2 L= o e = µe cN 2 = µe Lo = AL N 2 (H) (17.12) A hence µe = L 2 = L L (17.13) cN o where Lo is the coil inductance if the core is removed, whence the permeability drops. The term AL is the inductance factor and is equal to µe c. Conversely N =α L (17.14) where α = 1/√ AL and is termed the turns factor.
The effective permeability for high flux densities is expressed in terms of the amplitude permeability, µa, that is 1 1 ε (17.17) = + µe µa le That is
µa ε µa
A fringing factor, ε/β, must be introduced for significant gap widths, to account for the effective increase in permeability due to the fringing flux effect.
17.3.2v - Complex permeability, µ Because of core losses, a coil can be represented by • a series Ls - Rs circuit for an inductor • a parallel Rp // Lp circuit for a transformer. Core losses are modelled by the inclusion of resistance and the associated losses can be accounted for by considering the coil permeability as a complex variable, µ . For the inductor series equivalent circuit (17.19) Z = Rs + jω Ls = jωµ c N 2 (Ω) such that
µ = µ s' − j µ s" Ls Rs −j ω cN 2 cN 2 while for the transformer parallel equivalent circuit 1 1 1 = + (S) Z R p jω Lp =
Figure 17.4. Variation of permeability with field strength.
If the air gap, ε, is small compared with the core of length, le, such that ε